1 Acta Oceanol. Sin., 07, Vol. 6, No., P DOI: 0.007/s Biogenic synthesis of silver nanoparticles using ginger (Zingiber officinale) extract and their antibacterial properties against aquatic pathogens YANG Nan, LI Fuyan, JIAN Tiancai, LIU Chongchong, SUN Hushan, WANG Lei *, XU Hui School of Life Sciences, Ludong University, Yantai 605, China School of Chemistry and Materials Science, Ludong University, Yantai 605, China Received February 07; accepted 6 April 07 The Chinese Society of Oceanography and Springer-Verlag Berlin Heidelberg 07 Abstract With the development of aquaculture, there is an urgent demand for an alternative antibacterial agent to reduce the drug resistance and environmental pollution caused by the abuse of antibiotics. Recently, silver nanoparticles (AgNPs) have been viewed as a novel type of antimicrobial agents due to their unique advantages. In this study, AgNPs were biosynthesized with the ginger rhizomes extract. The biosynthesized AgNPs were characterised by UV visible spectroscopy, transmission electron microscopy, X-ray diffraction and fourier transform infrared spectroscopy. Furthermore, the antimicrobial activities of the AgNPs were fully analyzed against six typical aquatic pathogens. The results indicated that the components in ginger extract could function as the chemical reductant to synthesize AgNPs. Moreover, compared with the AgNPs synthesized by chemical methods, the biosynthesized AgNPs were smaller, and had higher stability and antibacterial activity. Therefore, the biosynthesized AgNPs using ginger extract may have prospective applications in aquaculture. Key words: ginger, silver nanoparticles, biosynthesis, antibacterial activity, aquatic pathogen Citation: Yang Nan, Li Fuyan, Jian Tiancai, Liu Chongchong, Sun Hushan, Wang Lei, Xu Hui. 07. Biogenic synthesis of silver nanoparticles using ginger (Zingiber officinale) extract and their antibacterial properties against aquatic pathogens. Acta Oceanologica Sinica, 6(): 95 00, doi: 0.007/s Introduction With the development of aquaculture, aquatic animal diseases caused by pathogens have become one of the biggest risk factors in the aquaculture industry (Francis et al., 00). Among these pathogens, a substantial proportion accounted for the conditions of pathogenic bacteria. Fish farmers have been forced to use antibiotics to inhibit the infections. However, abuse of antibiotics could not only pollute environment, but could also lead to serious drug resistance of pathogens on a very large scale (Schmidt et al., 000). Thus, there is an urgent demand for an alternative antibacterial agent to effectively control the aquatic pathogenic bacteria. As effective antibacterial agents, silver nanoparticles (AgNPs) have attracted much attention in the past decade (Martinez-Gutierrez et al., 00; Pavagadhi et al., 0). AgNPs can be synthesized by a variety of methods, among which chemical reduction are the most commonly used (Darroudi et al., 0). However, during the process, toxic chemicals are unavoidable as reducing agent and stabilising agent. Recently, the green synthesis of AgN- Ps has been developed via different biological systems, including bacteria, fungi, yeasts, algae or plants (Narayanan and Sakthivel, 00; Hebbalalu et al., 0; Miri et al., 05). The extracts from living organisms can act as reducing and stabilising agents. There are many advantages in the synthesis of AgNPs via biological extract, such as eco-friendliness, low cost, mild reaction conditions and compatibility for biomedical applications. Moreover, the bioactive compounds in the extract are supposed to improve the characteristics of the nanoparticles (NPs). For example, the proteins in Aspergillus oryzae var. viridis extracts could cap the AgN- Ps and prevent their aggregation (Binupriya et al., 00). Therefore, the biosynthesis of AgNPs would provide a new way for the development of novel antimicrobial agents. Ginger (Zingiber officinale) is not only a well-known spice plant, but also a traditional oriental medicine used to treat many diseases such as cough, nausea and vomiting, colds, rheumatism, cardiac disorders, inflammation and tumours (Leach and Kumar, 008; Dehghani et al., 0; Ding et al., 0). Ginger has been found to contain a variety of bioactive compounds, including alkaloids, flavonoids, zingiberene, gingerols and shogaols, most of which exhibit antioxidant activities (Shukla and Singh, 007; Park et al., 008; Butt and Sultan, 0). Given that ginger is rich in antioxidants, the biomolecules in ginger extract are supposed to play a crucial role in the reduction of silver ions (Ag + ) to metallic AgNPs (Ag 0 ). Velmurugan et al. (0) synthesized AgNPs using ginger root extract and proved their antimicrobial activity against food pathogens of Staphylococcus spp., Listeria spp. and Bacillus spp. However, to the best of our knowledge, there are no reports on antibacterial investigation of the ginger mediated AgNPs against aquatic pathogens. In this study, the AgNPs were biosynthesized with the aid of Foundation item: The Scientific Research Projects of Shandong University under contract No. J5LE0; the Key Research and Development Program of Shandong Province under contract No. 06GNC06; the Key Research and Developement Program of Yantai under contract No. 06ZH059. *Corresponding author,
2 96 YANG Nan et al. Acta Oceanol. Sin., 07, Vol. 6, No., P ginger extracts at moderate temperatures within a short period of time. Moreover, antibacterial analysis showed that the biosynthesized AgNPs exhibited powerful antimicrobial activities against all tested aquatic pathogens, which revealed their new potential in aquaculture field. Materials and methods. Materials The dried rhizomes of experimental material ginger (Z. officinale) were purchased from a local market of Yantai, China. The ginger was washed thoroughly with tap water followed by distilled water, shade-dried for a week and stored at C for further study. Silver nitrate (AgNO ) and sodium citrate (Na C 6 H 5 O 7 H O) were purchased from China National Pharmaceutical Group Corporation as analytical grade. Nutrient agar and nutrient broth were purchased from Sangon Biotech (Shanghai) Co., Ltd. Deionised water was used throughout the experimental procedure.. Chemical synthesis of AgNPs The AgNPs were prepared by chemical reduction. In brief, ml of 0.0 mol/l AgNO was added to 6 ml of deionised water. After the solution was boiled, ml of 0.00 g/ml sodium citrate was added drop by drop to the AgNO solution with constant stirring. Boiling was continued for h until the colourless mixed solution turned dark brown.. Biosynthesis of AgNPs Ginger extract was prepared by cutting 5.0 g of rhizome into small pieces, which were refluxed with 00 ml of 70% ethanol at 70 C for h. After cooling, the obtained extract was filtered through Whatman No. filter paper and centrifuged. The supernatant was collected and stored at C. For the biosynthesis of AgNPs, ml of ginger extract was added to 0 ml of the AgNO solution ( mmol/l) in a round-bottom flask. The mixture was heated at 85 C and color change of the solution was recorded within 0 min.. Characterization The as-prepared AgNPs were characterised by UV visible (vis) spectroscopy on a Shimadzu UV-550 spectrophotometer in the range of nm. The size and shape of AgNPs were analyzed by transmission electron microscopy (TEM, JEM 0) at an acceleration voltage of 00 kv. The freeze-dried powder of the resulting AgNP solution was used for X-ray diffraction (XRD; Rigaku D/max-500VPC) with Ni-filtered Cu Kα radiation at a scanning rate of 0.0 /s from 5 to 80. The Fourier transform infrared spectroscopy (FTIR) spectra of the samples were recorded by FTIR (Nicolet Nexus 670)..5 Antibacterial activity studies The antibacterial activity of the synthesized AgNPs was assayed by the agar well diffusion method (Wang et al., 06). Six typical aquatic pathogenic strains of Vibrio anguillarum, Vibrio alginolyticus, Aeromonas punctata, Vibrio parahaemolyticus, Vibrio splendidus and Vibrio harveyi (stored in the Department of Marine Biological Technology, Ludong University) were used to determine the antibacterial activity of the AgNPs. The test bacteria were cultivated at 8 C overnight in 6E liquid culture medium (tryptone 5.0 g/l, yeast extract.0 g/l, ferric phosphate 0. g/l, and seawater.0 L). About 00 μl of the bacterial culture suspensions with final concentrations of 0 6 cfu/ml (cfu is colony-forming units) was spread evenly on nutrient agar plates (tryptone 5.0 g/l, yeast extract.0 g/l, ferric phosphate 0. g/l, agar 5 g/l, and seawater.0 L). Oxford cups (8 mm in diameter) were gently placed on the inoculated agar plates, and 0 μl of the respective AgNPs samples was added to the cups. Sodium citrate and ginger extract served as controls. All plates were incubated at 8 C overnight. The zones of inhibition were measured and reported as an average. Experiments were performed in quadruplicate. Minimum inhibition concentration (MIC) of synthesized Ag- NPs was determined by broth dilution assay. V. anguillarum was chosen as the model organism. The samples were diluted and added to ml of 6E liquid culture medium with tested bacterial concentrations of 0 6 cfu/ml (the final concentration of the silver sample was µg/ml). The 6E medium was used as negative control and 0 6 CFU/mL bacterial suspensions as positive control. Bacterial growth was observed after h of incubation at 8 C. The lowest concentration of the prepared AgNPs at which no bacterial growth was observed in the culture suspensions was defined as the MIC. To ensure accuracy of results, the experiment was repeated three times. For the bacterial inhibition kinetic test, V. anguillarum was also selected as the index bacterium and incubated overnight at 8 C. The bacterial culture suspension was adjusted to 0 6 cfu/ml, and then the two obtained AgNPs as well as ginger extract and sodium citrate was added at a final concentration of 0 μg/ml, respectively. The bacteria solution was incubated at 8 C while being shaken at 50 r/min. Bacterial growth rates were measured by monitoring the optical density at 600 nm (OD 600 ) at different time intervals using a UV vis spectrophotometer (Shimadzu UV-550). Normal saline was used as control. To ensure accuracy of results, the experiment was repeated three times..6 Stability experiment The stability of the AgNP hydrocolloid was determined by visual inspection after 90 days of storage in C, followed by UV vis spectroscopy and the agar well diffusion method. Results and discussion. Characteristics of AgNPs We synthesized two kinds of AgNPs: by sodium citrate and by ginger extracts. As shown in Fig. a, the colour of the reaction solution changed to dark brown with sodium citrate and golden yellow with ginger extracts, indicating the formation of AgNPs (Fig. a). The colour change is attributed to the excited surface plasmon resonance (SPR) of the AgNPs and the colour depth is dependent on the concentration and size of the NPs (Mulvaney, 996). The formation of AgNPs was further examined by UV vis spectroscopy. As shown in Fig. b, the absorption spectrum of displayed a strong peak at 5 nm, whereas the at nm. Both of the characteristic peaks located in nm, which was the λ max range of typical AgN- Ps (Sadeghi and Gholamhoseinpoor, 05). These results indicated that the components in ginger extract could function as the chemical reductant to synthesize AgNPs. The morphology and size of the prepared AgNPs were evaluated by high-magnification TEM. The were heterogeneously dispersed with the size range of 0 80 nm, the majority of which were polygonally shaped (Fig. a). By contrast, were spherical and almost monodispersed with an average particle size of 0 nm (Fig. b). It is known that as for the AgNPs, the morphology and size are important criterions for any kind of
3 YANG Nan et al. Acta Oceanol. Sin., 07, Vol. 6, No., P b a ginger extracts sodium citrate sodium citrate solution Absorbance/a.u ginger extract Wavelength/nm Fig.. Production of AgNPs using sodium citrate and ginger extract (a), and UV vis absorption spectra of synthesized AgNPs (b). a b 50 nm 50 nm Fig.. TEM micrographs of (a) and (b). ans (Vidhu et al., 0). The calculated grain sizes of the and were about 8.7 nm and 9. nm, respectively, which were in agreement with the results of TEM analysis. The FTIR spectra of, and ginger extract in the range of cm were shown in Fig.. The ginger extract had peaks at 5.07, 99.8, 850.6, 6.78,., 75., 69., 8. and cm. Notably, the strong () Intensity/a.u. application (Panáček et al., 005). Previous studies also showed that spherical AgNPs with smaller size were anticipated to exhibit higher antibacterial properties (Pal et al., 007; Singh et al., 008). Hence, the results above indicated that the prepared were at an ideal state as antimicrobial agents. The crystalline structure of the synthesized AgNPs was investigated by XRD analysis (Fig. ). In the case of, four distinct diffraction peaks at θ=8.,., 6. and 77. corresponded to the (), (00), (0) and () planes of the facecentred cubic crystalline structure of Ag (JCPDS file No ). Thereby, the XRD pattern revealed that the sample was composed of crystalline face centered cubic (fcc) lattice structures of elemental silver. For, two weak peaks centred at θ of 8. and. were observed because of the low concentration of AgNPs, which was consistent with the aforementioned results of UV vis spectroscopy. Some of the unassigned diffraction peaks might be related to the crystallisation of bioorganic phases that attached to the surface of the NPs. The size of the NPs was thus determined based on Scherer s equation: (00) (a) (0) () (b) D = k λ / β cosθ, 0 where D is the average crystal size, k is the Scherer coefficient (0.89), λ is the X-ray wavelength (λ= m), θ is Bragg s angle (θ), β is the full width at half maximum (FWHM) in radi θ/( ) Fig.. XRD patterns of (a) and (b). 80
4 98 YANG Nan et al. Acta Oceanol. Sin., 07, Vol. 6, No., P at 99.8 and cm were caused by the C-H stretching vibrational mode, whereas the peaks at 6.8 and 75. cm were attributed to the C=O stretching vibration of aldehydes and flavonoid. The peak at 8. cm was attributed to the O-H deformation vibration of tertiary C-OH groups. Another weak peak near cm represented the C-O stretching vibration. The FTIR spectra of shared very similar absorption peak positions with that of the ginger extract, which indicated the presence of ginger extract on the surface of the AgNPs. Besides, the peaks both at 00 cm and 6.8 cm of the BAgNPs were obviously stronger than those of the, which further confirmed that the compounds in ginger extract interacted with the surface of AgNPs. Transmittance/% ginger extract Wavenumbers/cm Fig.. FTIR spectra of, and ginger extract. and wide band at 5.07 cm referred to the strong stretching vibrations of the O-H functional group. The corresponding peaks. Antimicrobial activities of synthesized AgNPs The antibacterial activity of synthesized AgNPs against six typical aquatic pathogens was evaluated by the agar well diffusion method. As shown in Fig. 5 and Table, sodium citrate solution did not produce any inhibition zone against the tested bacteria; the ginger extract and showed the inhibition zones which were slightly larger than the oxford cup, indicating Vibrio alginolyticus Vibrio anguillarum Aeromonas punctata Vibrio parahaemolyticus Vibrio splendidus Vibrio harveyi Fig. 5. Antibacterial effect of synthesized AgNPs against six different aquatic pathogens..,.,. sodium citrate solution, and. ginger extract.
5 YANG Nan et al. Acta Oceanol. Sin., 07, Vol. 6, No., P both of them had weak antibacterial activities. By contrast, B-Ag- NPs exhibited the significant inhibition zones against all of the tested bacteria, indicating that the had a broad spectrum of antibacterial activities and was promising in the treatment of aquatic pathogenic bacteria. For the MIC tests, gradiently diluted and C- AgNPs were incubated with equal volumes of V. anguillarum, respectively. After h of incubation, bacterial growth was studied by visual inspection. The MIC value of was defined as.9 μg/ml and was 50.0 μg/ml (Table ). The result indicated that showed relatively higher antibacterial activity than. Table. Diameter of inhibition zone (mm) of the synthesized AgNPs against various aquatic pathogenic bacteria Inhibition zone Pathogenic bacteria Test Control Sodium citrate Ginger extract Vibrio anguillarum 8.± ±0.05 NA 8.±0.9 Vibrio alginolyticus 8.8±0.09.±0.0 NA 8.0±0.00 Aeromonas punctata 8.5±0.0.5±0.07 NA 8.5±0. Vibrio parahaemolyticus 8.8±0.0.9±0.09 NA 8.±0. Vibrio splendidus 8.±0.08.±0.0 NA 8.±0.09 Vibrio harveyi 8.±0.0.6±0.0 NA 8.±0. Note: Values are expressed as the mean±standard error of the mean (n=). NA means not appearing. Table. Comparison of the MIC values of different samples (n=) Concentration of Ag/μg ml Sodium citrate Ginger extract Furthermore, antibacterial activity kinetics for the silver nanoparticles samples as well as ginger extract and sodium citrate toward V. anguillarum were studied. The 0 μg/ml of each sample was incubated in bacterium suspensions, and bacterial growth rate was monitored by measuring the optical density of the culture solution at various time intervals (Fig. 6). For the negative control of normal saline, the optical density increased rapidly during the bacteria log phase, indicating the reproduction of V. anguillarum. The sodium citrate shared a similar growth curve of V. anguillarum with the negative control, while both and ginger extract caused a growth delay of V. anguillarum and the growth curve increased gradually with a longer lag phase. Notably, V. anguillarum was completely inhibited as the optical density was almost the constant when treated with 0 μg/ml B- AgNPs. These results confirmed that the prepared had powerful antibacterial activities against the aquatic pathogen. AgNPs have been found to attach to the surface of the bacterial membrane, cause structural changes of the membrane, and finally lead to death of the microbe cells (Sondi and Salopek- Sondi, 00; Kim et al., 007). Generally, smaller AgNPs have a greater ability to penetrate cell membrane, and thus improve antibacterial activity (Singh et al., 008; Dubey et al., 00). In this study, with smaller and more uniform size possessed significantly higher antibacterial activity than, which is consistent with the previous reports. Besides, as the previous studies, the bioactive compounds in the ginger extract are supposed to improve the characteristics of the, thereby partially contributing to the higher antibacterial activities of B-AgN- Ps (Niraimathi et al., 0). OD (600 nm) µg/ml 0 µg/ml 0 µg/ml ginger extract 0 µg/ml sodium citrate normal saline Time/min Fig. 6. Growth curve of V. anguillarum in 6E media. C-AgN- Ps,, ginger extract and sodium citrate (0 μg/ml) was added into the culture, respectively.. Stability study The stability of AgNPs is a key factor that determines their antibacterial activity (Teeguarden et al., 007). Thus, we further evaluated the stability of and after 90 days. The UV vis absorption spectra showed that an obvious red-shift was observed in the surface plasmon peak of, while the shift was almost negligible in that of (Fig. 7). The results indicated that were agglomerated and were still well dispersed after 90 days. In addition, still showed remarkable diffusion zones against the tested aquatic pathogens after 90 days, whereas no longer produced inhibition zones (data not shown). Velmurugan et al. (0) proved that the existence of phenolic compounds, terpenoids and proteins in ginger extract may prevent agglomeration and
6 00 YANG Nan et al. Acta Oceanol. Sin., 07, Vol. 6, No., P Absorbance/a.u Wavelength/nm new synthesized new synthesized (90 days) (90 days) Fig. 7. Stability analysis of and stored for 90 days by UV vis spectroscopy. enhance stabilisation by covering the NPs. Therefore, the utilization of ginger extract during NP synthesis is beneficial to the stability of. Conclusions In this study, and were synthesized by ginger extracts and sodium citrate, respectively. TEM studies revealed that were superior to in either size or morphology. XRD and FTIR analyses confirmed that the active components of ginger extract could reduce Ag + and stabilize the AgNPs. Moreover, the showed higher antibacterial activities against aquatic pathogens than. Besides, B- AgNPs maintained better dispersion and higher stability than C- AgNPs after 90 days. Our results indicated that the ginger extract could effectively synthesize the AgNPs at moderate temperature, and this eco-friendly method may have prospective applications in aquaculture. References Binupriya A R, Sathishkumar M, Yun S I. 00. Myco-crystallization of silver ions to nanosized particles by live and dead cell filtrates of Aspergillus oryzae var. viridis and its bactericidal activity toward Staphylococcus aureus KCCM 56. Industrial & Engineering Chemistry Research, 9(): Butt M S, Sultan M T. 0. Ginger and its health claims: molecular aspects. Critical Reviews in Food Science and Nutrition, 5(5): 8 9 Darroudi M, Ahmad M B, Zak A K, et al. 0. Fabrication and characterization of gelatin stabilized silver nanoparticles under UVlight. International Journal of Molecular Sciences, (): Dehghani I, Mostajeran A, Asghari G. 0. In vitro and in vivo production of gingerols and zingiberene in ginger plant (Zingiber officinale Roscoe). Iranian Journal of Pharmaceutical Sciences, 7(): 7 Ding Mingshuang, Leach M J, Bradley H. 0. A systematic review of the evidence for topical use of ginger. EXPLORE: The Journal of Science and Healing, 9(6): 6 6 Dubey S P, Lahtinen M, Sillanpää M. 00. Green synthesis and characterizations of silver and gold nanoparticles using leaf extract of Rosa rugosa. Colloids and Surfaces A: Physicochemical and Engineering Aspects, 6( ): Francis G, Makkar H P S, Becker K. 00. Antinutritional factors present in plant derived alternate fish feed ingredients and their effects in fish. Aquaculture, 99( ): 97 7 Hebbalalu D, Lalley J, Nadagouda M N, et al. 0. Greener techniques for the synthesis of silver nanoparticles using plant extracts, enzymes, bacteria, biodegradable polymers, and microwaves. ACS Sustainable Chemistry & Engineering, (7): 70 7 Kim J S, Kuk E, Yu K N, et al Antimicrobial effects of silver nanoparticles. Nanomedicine, (): 95 0 Leach M J, Kumar S The clinical effectiveness of Ginger (Zingiber officinale) in adults with osteoarthritis. International Journal of Evidence-Based Healthcare, 6(): 0 Martinez-Gutierrez F, Olive P L, Banuelos A, et al. 00. Synthesis, characterization, and evaluation of antimicrobial and cytotoxic effect of silver and titanium nanoparticles. Nanomedicine, 6(5): Miri A, Sarani M, Bazaz M R, et al. 05. Plant-mediated biosynthesis of silver nanoparticles using Prosopis farcta extract and its antibacterial properties. Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, : 87 9 Mulvaney P Surface Plasmon spectroscopy of nanosized metal particles. Langmuir, (): Narayanan K B, Sakthivel N. 00. Biological synthesis of metal nanoparticles by microbes. Advances in Colloid and Interface Science, 56( ): Niraimathi K L, Sudha V, Lavanya R, et al. 0. Biosynthesis of silver nanoparticles using Alternanthera sessilis (Linn. ) extract and their antimicrobial, antioxidant activities. Colloids and Surfaces B: Biointerfaces, 0: 88 9 Pal S, Tak Y K, Song J M Does the antibacterial activity of silver nanoparticles depend on the shape of the nanoparticle? A study of the gram-negative bacterium Escherichia coli Applied and Environmental Microbiology, 7(6): 7 70 Panáček A, Kvítek L, Prucek R, et al Silver colloid nanoparticles: synthesis, characterization, and their antibacterial activity. The Journal of Physical Chemistry B, 0(): Park M, Bae J, Lee D S Antibacterial activity of -gingerol and -gingerol isolated from ginger rhizome against periodontal bacterial. Phytotherapy Research, (): 6 9 Pavagadhi S, Sathishkumar M, Balasubramanian R. 0. Uptake of Ag and TiO nanoparticles by zebrafish embryos in the presence of other contaminants in the aquatic environment. Water Research, 55: 80 9 Sadeghi B, Gholamhoseinpoor F. 05. A study on the stability and green synthesis of silver nanoparticles using Ziziphora tenuior (Zt) extract at room temperature. Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, : 0 5 Schmidt A S, Bruun M S, Dalsgaard I, et al Occurrence of antimicrobial resistance in fish-pathogenic and environmental bacteria associated with four Danish rainbow trout farms. Applied and Environmental Microbiology, 66(): Shukla Y, Singh M Cancer preventive properties of ginger: a brief review. Food and Chemical Toxicology, 5(5): Singh M, Singh S, Prasad S, et al Nanotechnology in medicine and antibacterial effect of silver nanoparticles. Digest Journal of Nanomaterials and Biostructures, (): 5 Sondi I, Salopek-Sondi B. 00. Silver nanoparticles as antimicrobial agent: a case study on E. coli as a model for Gram-negative bacteria. Journal of Colloid and Interface Science, 75(): 77 8 Teeguarden J G, Hinderliter P M, Orr G, et al Particokinetics in vitro: dosimetry considerations for in vitro nanoparticle toxicity assessments. Toxicological Sciences, 95(): 00 Velmurugan P, Anbalagan K, Manosathyadevan M, et al. 0. Green synthesis of silver and gold nanoparticles using Zingiber officinale root extract and antibacterial activity of silver nanoparticles against food pathogens. Bioprocess and Biosystems Engineering, 7(0): 95 9 Vidhu V K, Aromal S A, Philip D. 0. Green synthesis of silver nanoparticles using Macrotyloma uniflorum. Spectrochimica Acta Part A: Molecular and Biomolecular Spectroscopy, 8(): 9 97 Wang Lei, Liu Chongchong, Wang Yiyan, et al. 06. Antibacterial activities of the novel silver nanoparticles biosynthesized using Cordyceps militaris extract. Current Applied Physics, 6(9):